thermal destruction of metal-containing nanocomposites based on isotactic 342 thermal destruction of
Post on 27-May-2020
Embed Size (px)
"Science Stays True Here" Biological and Chemical Research, 341-358 | Science Signpost Publishing
Thermal Destruction of Metal-Containing
Nanocomposites Based on Isotactic Polypropylene
N. I.Kurbanova1, N.A. Alimirzoeva1, A. M. Kuliev1, T. I. Medintseva2, O. P. Kuznetsova2, E. V. Prut2 1. Institute of polymer materials of Azerbaijan national Academy of Sciences, Sumgayit.
2. Institute of chemical physics. n.a. N. N. Semenov of Russia Academy of Sciences, Moscow.
Received: August 22, 2016 / Accepted: September 20, 2016 / Published: November 25, 2016
Abstract: Created new thermoplastic elastomers based on isotactic polypropylene and ternary ethylene-propylene-diene
elastomer using a metal-containing nanofillers. Studied the influence of nanofillers containing nanoparticles of different
metals oxides on the physico-mechanical and thermal properties, as well as the structure of the uncured and
dynamically vulcanized blendsusing differential scanning calorimetry (DSC), differential thermal analysis (DTA) and
scanning electron microscope (SEM). Shown the emergence in the polymer containing metal nanoparticles, a fine
spherulitic structure, promoting the improvement of properties of obtained nanocomposites.
Key words: Thermoplastic elastomers, isotactic polypropylene, triple ethylene-propylene-diene elastomer, the
metal-containing nanofillers, DTA - DSC analysis
One of the most promising directions of development of modern science is nanotechnology – the
production and use of materials consisting of nanoparticles.
Considerable attention paid to the nanomaterials has been caused by at least two reasons. First, the
reduction in size is a traditional way to improve such material properties as catalytic activity and activity in
solid-phase reactions. Second, the unique physical properties of nanomaterials has been determined,
primarily magnetic and electrophysical [1-3].
The development of nanotechnology opened up t he possibility of conducting research in the area of
composite nanomaterials, and currently is allowed for the development and use of advanced polymer
materials for sensors, catalysis, nano-electronics etc. [4-6].
Corresponding author: N. I.Kurbanova, Institute of polymer materials of Azerbaijan national Academy of Sciences,
Thermal Destruction of Metal-Containing Nanocomposites Based on Isotactic Polypropylene 342
It is known that for improving of performance of plastics applied fillers in the amount of 30-50 wt.%.
Filled plastics are used mainly as structural material .
In the world today different types of polymer nanofiller-based composites are actively replacing
traditional materials . Polymer nanocomposites can be obtained in situ, i.e., by the polymerization of
monomer in presence of pre-dispersed in the reaction medium of the nanofiller . The method of
introduction of nanofillers in molten polymers is more preferred. This method is most suitable for use in
modern industry. It allows to obtain nanocomposite polymers to a wide range of manufacturers, which makes
this method promising and cost effective .
Modification of polypropylene by creating a variety of composite materials allows to significantly
expand the scope of its application. Filled polypropylene is one of the first places among the filled
thermoplastics. At present, more attention is paid to the development of composites with nanosized fillers.
Such composite materials have higher parameters than the composite materials with micro - and macrofillers.
Introduction into the polypropylene even of a small amount of nanoscale filler could significantly change the
physical properties, improve barrier performance, enhance thermal stability, electrical conductivity, etc [11,
The use of metal nanoparticles of variable valency (copper, cobalt, nickel, etc.) in polymers allows
to obtain fundamentally new materials that find wide application in radio - and optoelectronics as magnetic,
electro-conductive and optical media [5, 12].
Intensive development of the global petrochemical industry involves a constant search for a new
materials with high application properties, environmental safety and ease of processing. Such materials are
not without reason are thermoplastic elastomers (TPE). The creation of a TPE – is a priority direction of
work in the field of polymer materials science. Distinguishing feature of TPE is a combination of properties
of vulcanized rubbers during operation and thermoplastics during processing. [13-15].
The most promising approach to obtaining new types of TPE is mixing of elastomers with plastics with
simultaneous vulcanization of the elastomer. This leads to a high degree of dispersion of the rubber phase in
the obtained thermoplastic vulcanizers. Obtained by this method, the TPE has received the name of dynamic
thermoplastic elastomers (TPV). Due to the complex of high physical-mechanical properties, a w ide
temperature range of performance, lower cost of end products, TPV are considered one of the most
promising classes of polymer composite materials [16, 17].
There are works on obtaining of TPE and TPV with use of isotactic polypropylene(PP) as a thermoplast,
and of triple ethylene-propylene-diene elastomer (EPDM) or butadiene-nitrile rubber (NBR) as elastomers
Thermal Destruction of Metal-Containing Nanocomposites Based on Isotactic Polypropylene 343
using a variety of fillers or compatibilizators to improve the compatibility as well as physico-mechanical and
technological properties of the compositions [18-20].
Previously, we studied the effect of small additions of nanofillers (NF), containing nanoparticles (NPs)
of oxides of copper, nickel and iron, stabilized in polymer matrix, on t he features of properties of
thermoplastic elastomer mixed (TPE) and dynamically vulcanized (TPV) based on isotactic polypropylene
(PP) and ethylene-propylene-diene elastomer (EPDM). It is shown that a small addition of NF in the amount
of 1 weight part has virtually no effect on the crystallinity and dielectric permittivity of the TPE and TPV,
but reduces their elastic modulus. The obtained data of the electrical properties of TPE match those of
conventional dielectrics [21-22].
The work purpose - analysis of influence of additives for metal-containing nanofillers on the specifics
of thermophysical and thermal properties, as well as structure of mixed TPE and dynamically vulcanized
TPV based on isotactic PP and EPDM.
2. Materials and Research Methods
In the work has been used: isotactic polypropylene (PP) grade 21030-16 (Russia) with MP=7.7х104 and
Mw=3.4xl05; density p=0.907 g/cm3; the degree of crystallinity of 55%; melting temperature TM=165°C;
MFI=2.3 g/10 min at T=190°C and load 2.16 kg; brand EPDM Dutral TER 4044 (EPDM) with the number
of propylene units of 35%, a Mooney viscosity of 44 ( at 100°C); In the composition of the EPDM diene
component was 5-ethyliden-2 - norbornene in the amount of 4-5%.
As nanofillers (NF) used nanoparticles (NPs) of metal oxides , stabilized in polymer matrix: (NF-1) –
NPs of copper oxide I (Cu2O) and (NF-2) - nickel oxide (NiO) was stabilized in the matrix of the
polyethylene obtained with the use of titanium-phenolate catalytic system in the amount of 1 wt.% on the
polymer mixture. The content of nanoparticles in the polymer matrix: NPs of copper oxide - 3.9%, NPs of
nickel oxide - 18%, NPS size 11-15 nm, the degree of crystallinity of the NPs 25-45%.
The ratio of the initial components (mass.p.): PP/EPDM/NF = 50/50/1, Polymer composites are
obtained by mixing in a high-speed mixer of a closed type Brabender at T=190°C and rotor speed of 100
rp/m for 10 min, and vulcanized – by the method of dynamic vulcanization at the same conditions with the
use of sulfur-containing curing system comprising the following ingredients (in wt.p. on 100 wt. p. of
rubber): elemental sulfur 1.00, 2.50 zinc oxide, 1.00 stearic acid, di(2-benzothiazolyl)disulfide 0.25, the
tetramethylthiuramdisuphide 0.73 . Samples for testing were obtained by hot pressing in the form of
plates with a thickness of 0.35 mm at 190°C and a pressure of 10 MPa for 10 min followed by cooling to
room temperature at a speed of 20 deg /min.
Thermal Destruction of Metal-Containing Nanocomposites Based on Isotactic Polypropylene 344
For the study of mechanical characteristics of polymer mixtures from hotpressed plates were cut
samples in the form of blades with dimensions of 35.00x5.00x0.35 mm. Uniaxial tension of the specimens
was performed on test machine "Instron-1122" at room temperature and a constant rate of displacement of
the upper crosshead of 50 mm/min. From the diagrams of deformation by the initial part of the curve was
determined the modulus of elasticity E, ultimate strength σр and elongation at fracture EP. The results were
averaged by 10-14 samples. The error of measurement of elastic modulus and of ultimate strength did not
exceed 10%, and elongation at fracture -20%. The melt flow index (MFI) was determined on capillary